### Delft University of Technology

### Current-Phase Relation of Ballistic Graphene Josephson Junctions

Nanda, G.; Aguilera-Servin, J. L.; Rakyta, P.; Kormányos, A.; Kleiner, Reinhold; Koelle, Dieter; Watanabe, K.; Taniguchi, T.; Vandersypen, L. M.K.; Goswami, S.

DOI

10.1021/acs.nanolett.7b00097 Publication date

2017

Document Version Final published version Published in

Nano Letters: a journal dedicated to nanoscience and nanotechnology

Citation (APA)

Nanda, G., Aguilera-Servin, J. L., Rakyta, P., Kormányos, A., Kleiner, R., Koelle, D., Watanabe, K.,

Taniguchi, T., Vandersypen, L. M. K., & Goswami, S. (2017). Current-Phase Relation of Ballistic Graphene Josephson Junctions. Nano Letters: a journal dedicated to nanoscience and nanotechnology, 17(6), 3396-3401. https://doi.org/10.1021/acs.nanolett.7b00097

Important note

To cite this publication, please use the final published version (if applicable). Please check the document version above.

Copyright

Other than for strictly personal use, it is not permitted to download, forward or distribute the text or part of it, without the consent of the author(s) and/or copyright holder(s), unless the work is under an open content license such as Creative Commons. Takedown policy

Please contact us and provide details if you believe this document breaches copyrights. We will remove access to the work immediately and investigate your claim.

This work is downloaded from Delft University of Technology.

### Current-Phase Relation of Ballistic Graphene Josephson Junctions

### G. Nanda,

†### J. L. Aguilera-Servin,

†,∞### P. Rakyta,

¶### A. Korma

### ́nyos,

§### R. Kleiner,

∥### D. Koelle,

∥### K. Watanabe,

⊥### T. Taniguchi,

⊥### L. M. K. Vandersypen,

†,#### and S. Goswami

### *

,†,#†_{Kavli Institute of Nanoscience, Delft University of Technology, 2600 GA Delft, The Netherlands}
∞_{Institute of Science and Technology Austria, Am Campus 1, A-3400 Klosterneuburg, Austria}

¶_{Department of Physics of Complex Systems, Eo}_{̈tvös University, Pázmány Péter Sétány 1/A, H-1117 Budapest, Hungary}
§_{Department of Physics, University of Konstanz, D-78464 Konstanz, Germany}

∥_{Physikalisches Institut and Center for Quantum Science (CQ) in LISA+, Eberhard Karls Universita}_{̈t Tübingen, Auf der Morgenstelle}

14, D-72076 Tübingen, Germany

⊥_{National Institute for Materials Science, 1-1 Namiki, Tsukuba, 305-0044, Japan}
#_{QuTech, Delft University of Technology, 2600 GA Delft, The Netherlands}

### *

S Supporting InformationABSTRACT: The current-phase relation (CPR) of a Josephson junction (JJ) determines how the supercurrent evolves with the superconducting phase diﬀerence across the junction. Knowledge of the CPR is essential in order to understand the response of a JJ to various external parameters. Despite the rising interest in ultraclean encapsulated graphene JJs, the CPR of such junctions remains unknown. Here, we use a fully gate-tunable graphene superconducting quantum intereference device (SQUID) to determine the CPR of ballistic graphene JJs. Each of the two JJs in the SQUID is made with graphene encapsulated in hexagonal boron nitride. By independently controlling the critical current of the JJs, we can operate the SQUID either in a symmetric or asymmetric conﬁguration. The highly asymmetric SQUID allows us to phase-bias one of the JJs and thereby directly obtain its CPR. The CPR is found to be skewed, deviating signiﬁcantly from a sinusoidal form. The skewness can be tuned with the gate voltage and oscillates in antiphase with Fabry-Pérot resistance oscillations of the ballistic graphene cavity. We compare our experiments with tight-binding calculations that include realistic graphene−superconductor interfaces and ﬁnd a good qualitative agreement.

KEYWORDS: Graphene, Josephson junctions, SQUID, current-phase relation

### T

he past few years have seen remarkable progress in the study of graphene-superconductor hybrids. This surge in interest has primarily been driven by the ability to combine high-quality graphene with superconductors via clean interfaces and has led to several experimental advances. These include the observation of specular Andreev reﬂection,1 crossed Andreev reﬂections,2 and superconducting proximity eﬀects in ballistic graphene Josephson junctions (JJs).3−7 In a majority of these studies the device comprises of graphene encapsulated in hexagonal boron nitride (BN) contacted along the edge by a superconductor. The encapsulation in BN keeps the graphene clean, while the edge contacting scheme provides transparent interfaces. In particular, ballistic JJs fabricated in this manner have been central to recent studies of novel Andreev bound states in perpendicular magnetic ﬁelds,4 edge-mode super-conductivity,5and supercurrents in the quantum Hall regime.6 However, to date there have been no measurements of the Josephson current phase relation (CPR) in these systems.The CPR is arguably one of the most basic properties of a JJ and provides information about the Andreev bound state (ABS) spectrum in the junction. While typical super-conductor−insulator−superconductor (SIS) JJs exhibit a sinus-oidal CPR, deviations from this behavior can be present in superconductor−normal−superconductor (SNS) junctions. Examples of this include JJs with high transmission such as nanowires8,9 and atomic point contacts,10,11 where the CPR contains signiﬁcant higher frequency components. Further-more, the periodicity of the CPR itself can be diﬀerent from 2π for more exotic systems such as topological JJs.12For graphene JJs, there have been several numerical estimates of the CPR which take into account its linear dispersion relation.13−17More recently, ballistic graphene JJs operated in large magneticﬁelds Received: January 9, 2017

Revised: May 3, 2017 Published: May 5, 2017

Letter pubs.acs.org/NanoLett This is an open access article published under a Creative Commons Non-Commercial No

Derivative Works (CC-BY-NC-ND) Attribution License, which permits copying and redistribution of the article, and creation of adaptations, all for non-commercial purposes.

have been predicted to undergo a topological transition,18 which should be detectable via direct CPR measurements. However, the experimental determination of the CPR in graphene has been restricted to junctions that are either in the diﬀusive limit19 or in a geometry that does not allow gate control of the junction properties.20

Here, we use a direct current (dc) superconducting quantum interference device (SQUID) to directly determine the CPR in encapsulated graphene JJs. These graphene SQUIDs stand out from previous studies21,22 in two important ways. First, the superconducting contacts are made with molybdenum rhenium (MoRe), which allows us to operate the SQUID up to 4.2 K. More importantly, our SQUID consists of graphene JJs that are ballistic and independently tunable, thereby allowing full electrostatic control over the SQUID response. By applying appropriate gate voltages we can continuously tune from a symmetric to an asymmetric SQUID. We show that the asymmetric conﬁguration allows us to directly extract the CPR from ﬂux periodic oscillations in the critical current of the SQUID. The CPR is found to be nonsinusoidal, displaying a prominent forward skewing. This skewness can be tuned over a large range with the gate voltage and shows correlations with Fabry-Pérot (FP) resistance oscillations in the ballistic cavity. We complement our experiments with tight-binding simu-lations that go beyond the short junction limit and explicitly take into account realistic graphene−superconductor interfaces.

Figure 1a shows a scanning electron micrograph and cross-sectional schematic of a device. It consists of two encapsulated graphene JJs contacted with MoRe, incorporated in a SQUID loop. The fabrication strategy is similar to earlier work3 and

further details are provided in theSupporting Information(SI). The left (L-JJ)/right (R-JJ) JJs can be tuned independently by applying voltages (VL/VR) to local top gates. The junctions are

intentionally designed to have a geometrical asymmetry, which ensures that the critical current of R-JJ (IcR) is larger than that

of L-JJ (IcL) at the same carrier density. We report on two

devices (Dev1 and Dev2) both of which have the same lithographic dimensions (L × W) for L-JJ (400 nm × 2 μm). The dimensions of R-JJ for Dev1 and Dev2 are 400 nm× 4 μm and 400 nm × 8 μm, respectively. All measurements were performed using a dc current bias applied across the SQUID in a dilution refrigerator with a base temperature of 40 mK.

Figure 1b shows the variation in the normal state resistance (R) of the SQUID with VLandVRatT = 4.2 K. The device was

biased with a relatively large current of 500 nA, which is larger than the critical current of the SQUID for most of the gate range. Figure 1c shows a single trace taken along the white dashed line of Figure 1b, where R-JJ is held at the charge neutrality point (CNP). We see clear FP oscillations on the hole (p) doped region due to the formation of n−p junctions at the superconductor−graphene interfaces.3,4 Furthermore, the criss-cross pattern seen in the lower left quadrant ofFigure 1b indicates that both graphene junctions are in the ballistic limit and that there is no cross-talk between the individual gates. We note that whenVR> 3 V the critical current of the SQUID (Ic)

is larger than the applied current bias, and a zero-resistance state is thus visible even at 4.2 K. Having established the fact that our JJs are in the ballistic regime, we now look in more detail at the behavior of the SQUID. AtT = 4.2 K, we ﬁrst tune the gate voltages (VL = +10 V, VR = +2.5 V) such that the

Figure 1.(a) Scanning electron micrograph of the graphene dc-SQUID (Dev1) along with a cross-sectional schematic. Gate voltagesVLandVR

independently control the carrier density of the left and right junction, respectively. (b) Resistance R across the SQUID versus VL and VR,

demonstrating independent control of carrier type and density in the JJs. The bias current (I) for these measurements was ﬁxed at 500 nA. (c) Line trace taken along the dashed white line in (b) showing Fabry-Pérot oscillations in the hole-doped regime. (d) Diﬀerential resistance dV/dI as a function of dc current biasI and magnetic ﬁeld B with the SQUID operated in a symmetric conﬁguration (VL= +10 V andVR= +2.5 V).

Flux-periodic oscillations are clearly visible with a slowly decaying envelope arising from the interference pattern of a single JJ. (e)V−I plots [extracted from (d)] for diﬀerent values of magnetic ﬂux Φ showing a nearly 100% modulation of the critical current. All measurements shown here are performed atT = 4.2 K.

Nano Letters Letter

DOI:10.1021/acs.nanolett.7b00097

Nano Lett. 2017, 17, 3396−3401

SQUID is in a symmetric conﬁguration and I_{cR}=IcL.Figure 1d

shows the variation in diﬀerential resistance dV/dI with current biasI and magnetic ﬁeld B, where we observe clear oscillations inIcwith magneticﬂux. In this conﬁguration, the modulation in

Icis nearly 100%, as seen by the individualV−I traces inFigure 1e. The slow decay in the maximum value ofIcarises due to the

(Fraunhofer) magneticﬁeld response of a single junction. The devices were designed such that this background was negligible around B = 0 (that is, the SQUID loop area was kept much larger than the JJ area). Minimizing this background is important for a reliable determination of the CPR, as we will see below.

We now turn our attention to theﬂux-dependent response of a highly asymmetric SQUID (IcR≫ IcL), a condition that can

be readily achieved by tuning the gate voltages appropriately. To outline the working principle of the device, we start with the assumption that both JJs have a sinusoidal CPR (a more general treatment can be found in theSI). So, the critical current of the SQUID can be written asIc=IcLsinθ + IcRsinδ, where θ (δ) is

the phase drop across L-JJ (R-JJ). When an external magnetic
ﬂux (Φ) threads through the SQUID loop, the ﬂux and phase
are related byδ − θ = 2πΦ/Φ_{0}, assuming the loop inductance
is negligible. Now, whenIcR≫ IcL the phase diﬀerence across

R-JJ is very close toπ/2. Thus, I_{c}(Φ) ≈ I_{cR}+IcLsin(2πΦ/Φ0+

π/2) and the ﬂux-dependence of Icdirectly represents the CPR

of L-JJ, that is,Ic(Φ) ≈ IcR+Is(ϕ), where Isis the supercurrent

through L-JJ andϕ is the phase drop across it. This principle of using an asymmetric SQUID to probe the CPR has been employed in the past for systems such as point contacts10,11and vertical graphene JJs,20 where an SIS junction (with a well-known sinusoidal CPR) was used as the reference junction. In our case, the reference junction is also a graphene JJ, where the CPR is not known a priori. We show (seeSI) that this does not

aﬀect our ability to probe the CPR, provided time reversal symmetry is not broken, meaning that the CPR satisﬁes the conditionIs(ϕ) = −Is(−ϕ).

23

Throughout the remainder of the text we use R-JJ as the reference junction (larger critical current), and L-JJ is the junction under study (smaller critical current).

Figure 2a shows the typical magnetic response of the asymmetric SQUID atT = 40 mK with VL=−4 V (ﬁxed) and

diﬀerent values of V_{R}. For the most asymmetric conﬁguration
(VR= +10 V)Icoscillates around aﬁxed value of roughly 6 μA

(IcR) with an amplitude of about 500 nA (IcL). Using the

arguments described above, thisIc(Φ) curve can be converted

to Is(ϕ), as shown in Figure 2b. Here Is is the normalized

supercurrent deﬁned as (Ic− IcR)/IcL. We note that there is an

uncertainty (less than one period) in the exact position of zero B. This, combined with the unknown CPR of the reference graphene JJ, makes it important to do this conversion carefully, and we describe the details in theSI. The CPR shows a clear deviation from a sinusoidal form, showing a prominent forward skewing (that is,Ispeaks atϕ > π/2). We deﬁne the skewness

of the CPR asS = (2ϕmax/π) − 1,

19

whereϕ_{max}is the phase for
which the supercurrent is maximum.

To be certain that we are indeed measuring the CPR of L-JJ, we perform some important checks. We keep IcL ﬁxed and

reduceIcR(by reducingVR).Figure 2a shows that reducingIcR

merely shifts theIc(Φ) downward and therefore does not aﬀect

the extracted CPR, as one would expect. Furthermore, we use the experimentally determined CPR (from Figure 2b), the junction asymmetry, and loop inductance as inputs for the resistively and capacitively shunted junction (RCSJ) model to Figure 2.(a) Variation ofIcwithΦ for VL=−4 V and VR= +10, +5,

and +3 V at 40 mK. Solid black lines are results from RCSJ simulations of the SQUID. (b) Variation of supercurrentIs= (Ic− IcR)/IcL with

phaseϕ extracted from the top curve in (a). ϕmaxindicates the phase at

which Is reaches a maximum and is noticeably diﬀerent from π/2,

indicating a forward skewed CPR.

Figure 3.(a) Variation of skewnessS as a function of carrier density n for Dev1 and Dev2. The larger geometric asymmetry of Dev2 (see text) allows one to reliably probe the CPR up to higher n-doping. Inset shows the variation ofIcLwith density. (b) Aﬁner scan for Dev2 shows

thatS oscillates with carrier density in the p-doped regime in antiphase with Fabry−Pérot oscillations in the resistance.

compute the expected SQUID response (seeSIfor details of the simulations). These plots (solid lines) show an excellent agreement between simulations and experiment, thus con ﬁrm-ing that the asymmetry of our SQUID is suﬃcient to reliably estimate the CPR of L-JJ. Furthermore, it shows that there are no signiﬁcant eﬀects of inductance in our measurements, which could potentially complicate the extraction of the CPR from Ic(Φ) in an asymmetric SQUID.24

To study the gate dependence of the CPR weﬁx VRat +10 V

(to maximize IcR) and study the change in S with VL (Figure 3a) for Dev1 and Dev2. TheSIshows theIs(ϕ) curves used to

extractS. For both devices we ﬁnd that S is larger on the n-side as compared to the p-side, showing a dip close to the CNP. We note that Dev2 allows us to probe the CPR up to a larger range on the n-side due to its larger geometric asymmetry (seeSIfor other measurements on Dev2). We expect the skewness to depend strongly on the total transmission through the graphene JJ, which should depend on (a) the number of conducting channels in the graphene, as well as (b) the transparency of the graphene-superconductor interface. The gate voltageVLobviously changes the Fermi wave vector but it

also changes the contact resistance,25which plays a signiﬁcant role in determiningS. This can be seen most clearly for Dev2 for high n-doping, where S saturates, despite the fact that IcL

continues to increase up to the largest measured density (see

inset). At large p-doping,S also seems to saturate but a closer look (Figure 3b) shows that S oscillates in antiphase with the FP oscillations in resistance. This clearly indicates that in this regime the CPR is modulated by phase coherent interference eﬀects similar to the FP oscillations that aﬀect the total transmission.

We complement our measurements with a minimal theoretical model by solving the corresponding Bogoliubov− de Gennes (BdG) equations to calculate the CPR in graphene JJs. To set the stage, we note that SNS junctions can be characterized by the quasiparticle mean free path lf in the

normal (N) region and the coherence length ξ0=ℏvF/Δ, where

vFis the Fermi velocity inN. In our devices L ≪ lf, that is, they

are in the ballistic regime, and therefore we neglect impurity scattering in our calculations. TakingvF≈ 106m/s for graphene

andΔ ≈ 1.2 meV for MoRe, one ﬁnds ξ0 = 548 nm, which

means that in our junctionsL ≲ ξ0, that is, they are not in the

strict short junction limitL ≪ ξ0. Consequently, the Josephson

current is carried not only by discrete Andreev bound states (ABSs) but also by states in the continuum (CONT).26−28For this reason, we numerically solve the BdG equations using a tight-binding (TB) model (see Figure 4a) and a recently developed numerical approach17,29which handles the ABSs and states in the continuum on equal footing. The description of both the normal region and the superconducting terminals is Figure 4.(a) The geometry of the system used in the calculations. The superconducting leads are attached in a top-contact geometry to the normal graphene sheet and overlap with the normal graphene sheet overNLunit cells.γ denotes the nearest-neighbor intralayer hopping in the leads and in

the graphene sheet, whileγ1is the nearest-neighbor interlayer hopping. A periodic boundary condition is applied in they-direction. (Inset) Top view

of the system. Because of doping from the S contacts, the normal graphene region is assumed to be n-doped up to a distancex1(x2) from the left

(right) contact. The distanceL* = x2− x1is the eﬀective cavity length which depends on the gate voltage applied to the junction. (b) The

contribution of the ABSs (red) and continuum CONT (blue) to the total supercurrent (black) as a function of the phase diﬀerence for an n-doped
junction (n = 0.9 × 1011_{cm}−2_{and}_{L/ξ}

0= 0.73). (c) The skewnessS as a function of doping of the junction. The regimes i−iii indicated by the

rectangles are further discussed in the text. Dashed lines show the averageS in the p- and n-doped regime. (d) The skewness (red circles, left axis) and normal state resistance (blue, right axis) versus doping for strong p-doping of the junction.

Nano Letters Letter

DOI:10.1021/acs.nanolett.7b00097

Nano Lett. 2017, 17, 3396−3401

based on the nearest-neighbor TB model of graphene.30 The on-site complex pair-potential Δ is ﬁnite only in the superconducting terminals and changes as a step-function at the N−S interface. The results presented here are calculated using the top-contact geometry (Figure 4a), a model with perfect edge contacts is discussed in the SI. As observed experimentally, we take into account n-doping from the superconducting contacts (seeFigure 4a inset). If the junction is gated into hole-doping, a FP cavity is formed by the two n−p junctions in the vicinity of the left and right superconducting terminals. The lengthL* of this FP cavity depends on the gate voltage,4for stronger hole-doping the n−p junctions shift closer to the contacts. For further details of the model seeSI.

Turning now to the CPR calculations, Figure 4b shows separately the contribution of the ABS and the continuum to the supercurrent. BecauseL ≲ ξ0, the latter contribution is not

negligible and aﬀects both the value of the critical current and the skewness of the CPR. We note that our calculations can qualitatively reproduce the doping dependence ofIc (seeSI),

however the obtained values of Ic are about 2.5 times larger

than the measurements (Figure 3a inset). The exact reason for this discrepancy is not known, but a similar disagreement between theory and experiment was also found in ref 4. Focusing now on the skewness, in Figure 4c we show the calculated skewness S as a function of the doping of the junction at zero temperature. We consider three regimes: (i) strongly p-doped junction; (ii) large n-doping, (iii) the region around the CNP. We start with the discussion of (i). It is well established that in this case the p−n junctions lead to FP oscillations in the normal resistance as well as in the critical current3,4of graphene JJs. Our calculations, shown inFigure 4d, indicate that due to FP interference the skewness also displays oscillations as a function of doping around an average value ofS ≈ 0.23. As already mentioned, similar oscillations are present in the normal state resistanceR, however, we ﬁnd that R oscillates in antiphase with the skewness. Compared to the measure-ments (Figure 3b), our calculations therefore reproduce the phase relation between the oscillations of the skewness andR and give a qualitatively good agreement with the measured values of the skewness. In the strong n-doped regime (case (ii) the calculated average skewness ofS = 0.27 is larger than for p-doped junctions, and very close to the measured values. Small oscillations ofS are still present in our results and they are due to the n−n′ interfaces, that is, the diﬀerence in the doping close to the contacts (forx < x1andx > x2, seeFigure 4a inset) and

the junction region (x1 < x < x2), which enhances

back-scattering. Our calculations therefore predict smaller skewness for p-doped than for n-doped junctions. The enhancement ofS in the n-doped regime can be clearly seen in the measurements ofFigure 3a. We note that previous theoretical work,16which calculated the spatial dependence of the pairing amplitude self-consistently, predicted a skewness of S ≈ 0.15 for n-doped samples with L < ξ0, while a nonself-consistent calculation

which took into account only the contribution of the ABS yieldedS ≈ 0.42.16The comparison of these results to ours and to the measurements suggest that the skewness may depend quite sensitively on theS−N interface as well as on the L/ξ0

ratio and that our approach captures the most important eﬀects in these junctions. Finally, we brieﬂy discuss the case (iii), where the measurements show a suppression of the skewness as the CNP is approached. The measured values of S ∼ 0.1 are similar to those found in diﬀusive junctions19 but are signiﬁcantly lower than the theoretical prediction of S = 0.26

in the short junction limit13at the CNP. This suppression ofS is not reproduced in our calculations, instead, we ﬁnd rapid oscillations as the CNP is approached from the p-doped regime. This discrepancy is likely to be due to eﬀects that are not included in our ballistic model, such as charged scatterers that are poorly screened in this regime, or scattering at the edges, which is more relevant at low densities when only a few open channels are present.

Finally, we study the eﬀect of temperature on the CPR of these JJs. In Figure 5a, we compare the CPR in the n-doped

regime (VL= +1 V;n = 0.9 × 1011cm−2) at 40 mK and 4.2 K.

One clearly sees that at 4.2 K the CPR is sinusoidal. This is consistent with our observation that the critical current modulation of the SQUID is nearly 100% at 4.2 K (Figure 1d), a condition which can only be achieved if the CPR is sinusoidal.Figure 5b shows the full temperature dependence of S for two representative values of electron and hole doping (see

SIfor the corresponding temperature dependence of the critical currents). The reduction in skewness with temperature is consistent with the thermal population of excited Andreev bound states and continuum states.14,16,17,19We compare our results with numerical estimates which take into account this eﬀect, along with the temperature dependence of the pair potential (black curves in Figure 5b). While the qualitative behavior of both (experimental and numerical) curves are Figure 5.(a) CPR forVL= +1 V (n = 0.9 × 1011cm−2) at 40 mK

(upper curve) and 4.2 K (lower curve). Solid line shows the calculated CPR. A forward skewness is clearly seen in the curve at 40 mK but is absent at 4.2 K. (b) Variation ofS with temperature for electron and hole doping. Increasing the temperature suppresses higher harmonics in the CPR, thereby reducingS until it vanishes near 4.2 K and the curves become sinusoidal. Black lines show the results of tight binding simulations.

similar, the experimentally determined skewness reaches zero (sinusoidal CPR) faster than the numerics. At this point, it is diﬃcult to ascertain the exact reason for this discrepancy but one possible explanation for this is that the induced superconducting gap in the graphene is somewhat smaller than the bulk MoRe gap, resulting in a faster decay.

In conclusion, we have used a fully gate-tunable graphene based SQUID to provide measurements of the current-phase relation in ballistic Josephson junctions made with encapsulated graphene. We show that the CPR is nonsinusoidal and can be controlled by a gate voltage. We complement our experiments with tight binding simulations to show that the junction length and nature of the superconductor−graphene interface play an important role in determining the CPR. We believe that the simplicity of our device architecture and measurement scheme should make it possible to use such devices for studies of the CPR in topologically nontrivial graphene Josephson junctions.

## ■

ASSOCIATED CONTENT### *

S Supporting InformationThe Supporting Information is available free of charge on the

ACS Publications website at DOI: 10.1021/acs.nano-lett.7b00097.

Device fabrication; additional data from other devices; magnetic ﬁeld to phase conversion; quantifying in-ductance eﬀects; RCSJ simulations; details of tight binding-Bogoliubov-de Gennes calculations (PDF)

## ■

AUTHOR INFORMATION Corresponding Author *E-mail:S.Goswami@tudelft.nl. ORCID J. L. Aguilera-Servin:0000-0002-2862-8372 S. Goswami:0000-0002-9095-4363 NotesThe authors declare no competingﬁnancial interest.

## ■

ACKNOWLEDGMENTSWe thank A. Geresdi and D. van Woerkom for useful discussions. S.G. and L.M.K.V. acknowledge support from the EC-FET Grapheneﬂagship and the Dutch Science Foundation NWO/FOM. A.K. acknowledges funding from FLAG-ERA through project“iSpinText”. P.R. acknowledges the support of the OTKA through the Grant K108676, the support of the postdoctoral research program 2015, and the support of the János Bolyai Research Scholarship of the Hungarian Academy of Sciences. K.W. and T.T. acknowledge support from the Elemental Strategy Initiative conducted by the MEXT, Japan and JSPS KAKENHI Grants JP26248061, JP15K21722, and JP25106006.

## ■

REFERENCES(1) Efetov, D. K.; Wang, L.; Handschin, C.; Efetov, K. B.; Shuang, J.; Cava, R.; Taniguchi, T.; Watanabe, K.; Hone, J.; Dean, C. R.; Kim, P. Nat. Phys. 2015, 12, 328−332.

(2) Lee, G. H.; Huang, K. F.; Efetov, D. K.; Wei, D. S.; Hart, S.; Taniguchi, T.; Watanabe, K.; Yacoby, A.; Kim, P.Nat. Phys. 2017, in pressDOI: 10.1038/nphys4084.

(3) Calado, V. E.; Goswami, S.; Nanda, G.; Diez, M.; Akhmerov, A. R.; Watanabe, K.; Taniguchi, T. M. K.; Vandersypen, L. M. K.Nat. Nanotechnol. 2015, 10, 761−764.

(4) Shalom, M. B.; Zhu, M. J.; Fal’ko, V. I.; Mishchenko, A.; Kretinin, A. V.; Novoselov, K. S.; Woods, C. R.; Watanabe, K.; Taniguchi, T.; Geim, A. K.; Prance, J. R.Nat. Phys. 2015, 12, 318.

(5) Allen, M. T.; Shtanko, O.; Fulga, I. C.; Akhmerov, A. R.; Watanabe, K.; Taniguchi, T.; Jarillo-Herrero, P.; Levitov, L. S.; Yacoby, A.Nat. Phys. 2015, 12, 128−133.

(6) Amet, F.; Ke, C. T.; Borzenets, I. V.; Wang, J.; Watanabe, K.; Taniguchi, T.; Deacon, R. S.; Yamamoto, M.; Bomze, Y.; Tarucha, S.; Finkelstein, G.Science 2016, 352, 966−969.

(7) Borzenets, I. V.; Amet, F.; Ke, C. T.; Draelos, A. W.; Wei, M. T.; Seredinski, A.; Watanabe, K.; Taniguchi, T.; Bomze, Y.; Yamamoto, M.; Tarucha, S.; Finkelstein, G.Phys. Rev. Lett. 2016, 117, 237002.

(8) Murani, A.; Kasumov, A.; Sengupta, S.; Kasumov, Y.; Volkov, V. T.; Khodos, I.; Brisset, F.; Delagrange, R.; Chepelianskii, A.; Deblock, R.; Bouchiat, H.; Guéron, S. 2016, arXiv:1609.04848, accessed January 9, 2017.

(9) Spanton, E. M.; Deng, M.; Vaitiekėnas, S.; Krogstrup, P.; Nygård, J.; Marcus, C. M.; Moler, K. A. 2017, arXiv:1701.01188, accessed January 9, 2017.

(10) Miyazaki, H.; Kanda, A.; Ootuka, Y. Phys. C 2006, 437-438, 217−219.

(11) Della Rocca, M. L.; Chauvin, M.; Huard, B.; Pothier, H.; Esteve, D.; Urbina, C.Phys. Rev. Lett. 2007, 99, 127005.

(12) Fu, L.; Kane, C. L.Phys. Rev. B: Condens. Matter Mater. Phys. 2009,79, 161408.

(13) Titov, M.; Beenakker, C. W. J.Phys. Rev. B: Condens. Matter Mater. Phys. 2006, 74, 041401.

(14) Hagymási, I.; Kormányos, A.; Cserti, J. Phys. Rev. B: Condens. Matter Mater. Phys. 2010, 82, 134516.

(15) Black-Schaffer, A. M.; Doniach, S.Phys. Rev. B: Condens. Matter Mater. Phys. 2008, 78, 024504.

(16) Black-Schaffer, A. M.; Linder, J.Phys. Rev. B: Condens. Matter Mater. Phys. 2010, 82, 184522.

(17) Rakyta, P.; Kormányos, A.; Cserti, J. Phys. Rev. B: Condens. Matter Mater. Phys. 2016, 93, 224510.

(18) San-Jose, P.; Lado, J.; Aguado, R.; Guinea, F.; Fernández-Rossier, J.Phys. Rev. X 2015, 5, 041042.

(19) English, C. D.; Hamilton, D. R.; Chialvo, C.; Moraru, I. C.; Mason, N.; Van Harlingen, D. J.Phys. Rev. B: Condens. Matter Mater. Phys. 2016, 94, 115435.

(20) Lee, G. H.; Kim, S.; Jhi, S. H.; Lee, H. J.Nat. Commun. 2015, 6, 6181.

(21) Girit, Ç.; Bouchiat, V.; Naaman, O.; Zhang, Y.; Crommie, M. F.; Zettl, A.; Siddiqi, I.Nano Lett. 2009, 9, 198.

(22) Girit, Ç.; Bouchiat, V.; Naaman, O.; Zhang, Y.; Crommie, M. F.; Zettl, A.; Siddiqi, I.Phys. Status Solidi B 2009, 246, 2568.

(23) Golubov, A. A.; Kupriyanov, M. Y.; Il’ichev, E. Rev. Mod. Phys. 2004,76, 411−469.

(24) Fulton, T. A.; Dunkleberger, L. N.; Dynes, R. C.Phys. Rev. B 1972,6, 855−875.

(25) Wang, L.; Meric, I.; Huang, P. Y.; Gao, Q.; Gao, Y.; Tran, H.; Taniguchi, T.; Watanabe, K.; Campos, L. M.; Muller, D. A.; Guo, J.; Kim, P.; Hone, J.; Shepard, K. L.; Dean, C. R.Science 2013, 342, 614− 617.

(26) Svidzinsky, A. V.; Antsygina, T. N.; Bratus, E. N.J. Low Temp. Phys. 1973, 10, 131.

(27) Giuliano, D.; Affleck, I.J. Stat. Mech.: Theory Exp. 2013, 2013, P02034.

(28) Perfetto, E.; Stefanucci, G.; Cini, M. Phys. Rev. B: Condens. Matter Mater. Phys. 2009, 80, 205408.

(29) The numerical calculations were performed with the EQuUs software, see http://eqt.elte.hu/equus/home, accessed January 9, 2017.

(30) Wakabayashi, K.; Fujita, M.; Ajiki, H.; Sigrist, M.Phys. Rev. B: Condens. Matter Mater. Phys. 1999, 59, 8271−8282.

## ■

NOTE ADDED AFTER ASAP PUBLICATIONThis paper published ASAP on 5/11/2017. Figure 3 was corrected and the revised version was reposted on 5/16/2017.

Nano Letters Letter

DOI:10.1021/acs.nanolett.7b00097

Nano Lett. 2017, 17, 3396−3401